1 Nanomaterials Volume 2015, Article ID , 7 pages Research Article Luminescence Properties of CaF 2 Nanostructure Activated by Different Elements Numan Salah, 1 Najlaa D. Alharbi, 2 Sami S. Habib, 3 ands.p.lochab 4 1 Center of Nanotechnology, King Abdulaziz University, Jeddah 21589, Saudi Arabia 2 Sciences Faculty for Girls, King Abdulaziz University, Jeddah 21589, Saudi Arabia 3 Department of Aeronautical Engineering, King Abdulaziz University, Jeddah 21589, Saudi Arabia 4 Inter-University Accelerator Centre, Aruna Asaf Ali Marg, New Delhi , India Correspondence should be addressed to Numan Salah; Received 29 September 2014; Accepted 9 December 2014 Academic Editor: Songjun Zeng Copyright 2015 Numan Salah et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Nanostructures of calcium fluoride (CaF 2 ) doped with Eu, Tb, Dy, Cu, and Ag were synthesized by the coprecipitation method and studied for their thermoluminescence (TL) and photoluminescence (PL) properties. The PL emission spectrum of pure CaF 2 nanostructure has a broad band in the nm range. Similar spectra were observed in case of doped samples, beside extra bands related to these impurities. The maximum PL intensity was observed in Eu doped sample. The TL results of Eu, Cu, Ag, and Tb doped samples show weak glow peaks below 125 C, whereas Dy doped one is found to be highly sensitive with a prominent peak at 165 C.Thissamplewasfurtherexposedtoawiderangeofgammaraysexposuresfrom 137 Cs source. The response curve is linear in the 100 Gy-10 kgy range. It is also observed that the particle size of CaF 2 nanostructure was significantly reduced by increasing Dy concentration. These results showed that Dy is a proper activator in the host of CaF 2 nanostructure, providing a highly sensitive dosimeter in a wide range of exposures and also plays a role as a controlling agent for particle size growth. 1. Introduction Nanoscale materials or nanostructures have attracted huge attention in the last two decades due to their unique properties. They have a potential to be used in a variety of applications. A large number of individuals and research groups from different fields have produced different nanomaterials and studied their properties. These include structural, optical, electrical, magnetic, mechanical, and dosimetric properties [1 5]. Many methods of preparations have also been developed in the last two decades, where different nanostructures like nanoparticles, nanocubes, nanowires, nanorods, and so forth, of several materials have been produced [6, 7]. Recent investigations have showed that the optical, luminescent, and other properties can be modified by the shape and size of the nanostructures. The role of impurity(ies) in the host of these nanostructure is another parameter that can be used to modify their properties [8 10]. Thermoluminescence (TL) is a well-known technique widely used for detection and measurement of absorbed radiation and dating of archaeological samples. It is a powerful technique for detecting defects in solid materials and dosimetry of different ionizing radiations. The presently used TL dosimeter (TLD) materials are inorganic crystalline materials mainly low Z effective compounds. However, the selected TLD materials have advantage and drawbacks; therefore, effortsarestillgoingontoimprovetheirdosimetricproperties. These improvements were tried to be achieved by either improving the TL characteristics of these TLD materials by preparing them using different methods or by doping with different impurities [11, 12]. Almost all of these phosphors have dose ranges depending on their TL sensitivity and response characteristics (linearity and saturation) to high energy radiations. In the last few years, Salah and his group have produced nanostructures of some highly sensitive phosphors [13 21]
2 2 Nanomaterials and studied their TL response to different ionizing radiations. They observed that these nanostructures have unique dosimetric properties, mainly their linear response over a wide range of exposures along with a negligible fading. These nanomaterials are insensitive to heat treatments, making themquiteusefultoestimatetheheavydosesofionizing radiations. These results are observed in tissue and nontissue equivalent nanomaterials [13 21]. Other workers have also participated in testing TL response of some nanostructure materials to different ionizing radiations [22 28]. These studies showed that the TL response of these nanomaterials to ionizing radiations is mostly linear in a wide range of exposures; however, few studies were focused on the TL response of low Z effective nanomaterials. Calcium fluoride (CaF 2 ) is a wide band gap material with a large-scale transparency. Therefore, color center formation is possible just by irradiating CaF 2 by ionizing radiation . The material has a relatively low Z effective, making it suitable for ionizing radiations used in radiotherapy. It was reported that this material is suitable as a laser material particularly, when doped with rare earth elements . The nanostructure form of CaF 2 was synthesized by different methods [29, 31 33]. However, the TL and PL properties of this nanomaterial have not been well studied. Few studies were focused on the effect of different dopants on its optical properties [34 36]. Other investigations were focused on different routes for the syntheses of CaF 2 nanocrystals and study of the upconversion luminescence by doping with some rare earths [37, 38]. In this work CaF 2 nanostructure particles were doped with different impurities and studied for their TL response to gamma rays in a wide range of exposures. The effect of dopant concentration on the particle shape and size of CaF 2 was also investigated (i.e., Dy in CaF 2 nanocubes). Pure and doped samples were synthesized by the coprecipitation method.theyweredopedwitheu,tb,dy,cu,andag.theas synthesized nanomaterials were characterized by XRD, SEM, DSC, and PL. Then they were exposed to a wide range of gamma rays exposures. 2. Experimental Pure, europium (Eu), dysprosium (Dy), terbium (Tb), silver (Ag) and copper (Cu) doped CaF 2 nanocrystalline samples were synthesized by the chemical coprecipitation method. The samples of CaF 2 were synthesized by using water and ethanol as solvents at a ratio of 1 : 1. The desired concentration of calcium chloride (CaCl 2 ) was dissolved in triply distilled DI water. The normality of the solution was kept at 0.2 N. This solution was mixed with ammonium fluoride (NH 4 F) solution (has a normality of 0.2 N). The solution of ammonium fluoride was added to that of calcium chloride dropwise with continuous stirring. The formed precipitate was filtered out andwashedwithdistilledwaterseveraltimes.theresulting powder samples, thus obtained, were dried at 70 Cinan oven for 3 hours. The used chemicals in this experiment are highlypureandwereofargrade.thedopantsusedinthis study were incorporated in their chloride forms except that of Ag dopant, where nitrate compound is used. A typical concentration of these impurities, that is, 0.2 mole%, is used in CaF 2 samples except those doped with Dy, where different concentrations in the range mole% are studied. In a typical case the desired concentration of the impurity, that is, DyCl 3 6H 2 O, was added to the solution of CaCl 2 and stirred for one hour before adding the solution of NH 4 Fas mentioned above. For TL study the produced samples were annealed at 350 Cfor1h. The samples of CaF 2 were characterized by X-ray diffraction (XRD), using an Ultima-IV (Rigaku, Japan) diffractometer with Cu Kα radiation, while the morphology of these samples was studied by a field emission scanning electron microscopy (FESEM), JSM-7500 F (JEOL, Japan). Photoluminescence (PL) emission spectra were recorded at an excitation wavelength of 325 nm using a fluorescence spectrofluorophotometer, model RF-5301 PC, Shimadzu, Japan. A cutofffilter(uv-39)isusedtoblocktheemissionsfromthe excitation source or scattered light. The PL measurement was conductedatroomtemperature.thestudyoftemperature behavior was studied under nonisothermal measurements by using a Shimadzu DSC-60 instrument. Typically, 5 mg of sampleinpowderformwassealedinstandardaluminum sample pans and heated at a heating rate of 10 C/min. The temperature precision of this equipment is ±0.1 K. Thermoluminescence (TL) glow curves were recorded on a Harshaw TLD reader (model 3500) under nitrogen atmosphere at a heating rate of 5 C/s. Neutral density filters of optimized density were used to avoid saturation of the photomultiplier tube (PMT) detector. For TL measurement 5 mg of sample was taken each time. The background reading is initially recorded and subtracted from the samples reading. 3. Results and Discussion Figure 1 shows SEM images at different magnifications ((a) and(b))ofpurecaf 2 sample. These images show a mixture of spherical and cubic shape structures. These structures have sizesintherangeof20 80nm.Theproducednanostructures have a good particle size distribution. As mentioned in Section 2 that the used compounds of CaCl 2 and NH 4 Fwere dissolved in water: ethanol mixture at a ratio of 1 : 1. This ratio was found to provide small nanostructures, while other ratios showed bigger particles. Figure 2 shows XRD pattern of the as-synthesized pure CaF 2 sample. Several diffracted peaks can be seen with hkl values indicating a complete crystalline structure in a cubic phase (JCPDS Card number ). The displayed peaks correspond to values (1 1 1), (2 2 0), (3 1 1), and (4 0 0). The XRD pattern presents broad peaks revealing the small crystallite size of the synthesized samples. This result is similar to that reported in the literature . The nanocrystalline size was calculated using Scherer s formula and found to be around 35 nm. This value is close to that observed by SEM (Figure 2). XRD of the doped samples was alsostudied,buttheresultissimilartothatofpurecaf 2 nanostructure. The concentration of these dopants used in this study was low, which is 0.2 mole%. At this concentration
3 Nanomaterials 3 (a) (b) (a) (b) Figure 1: SEM images of the as-synthesized CaF 2 nanostructures taken at different magnifications. 30 Intensity (111) (220) (311) (400) Angle (2θ) Figure 2: XRD pattern of the as-synthesized CaF 2 nanostructures. Exo Heat flow (mw) Endo Temperature ( C) Figure 3: DSC plot for the as-synthesized CaF 2 nanostructures. no significant changes are observed in the XRD peak of pure sample. DSC measurement for pure CaF 2 sample was conducted in the range of C. The DSC curve is shown in Figure 3. There is no endo- or exothermic peaks in this range, which means that pure CaF 2 has only a single phase. For the dosimetry using thermoluminescence technique, the material of the dosimeter should be thermally stable without any phase transitions in the range C. Figure 4 shows the PL emission spectra of the asproduced nanostructures of pure (curve (a)) and doped CaF 2 samples (curves (b) (f)). As mentioned above, the samples of CaF 2 nanostructures were doped with Ag, Eu, Tb, Cu, and Dy at a concentration of 0.2 mole% and their PL result is shown in curves (b), (c), (d), (e), and (f), respectively. Pure sample (curve (a)) shows a broad band in the nm range. This band might be induced due to the formation of color centers. These centers perhaps could be created by oxygen defects within the host of CaF 2.Ithasbeenreportedthat oxygen defects (contaminations) can induce such emission bands, but at the higher wavelength side of the visible region. In the present CaF 2 nanostructures, reducing the particle size PL intensity (a.u.) c f e d b a Wavelength (nm) (a) Pure CaF 2 (b) CaF 2 :Ag (c) CaF 2 :Eu (d) CaF 2 :Tb (e) CaF 2 :Cu (f) CaF 2 :Dy Figure 4: PL emission spectra of the as-synthesized nanostructures of pure and doped CaF 2 samples, doped with different impurities at a concentration of 0.2 mole%.
4 4 Nanomaterials tothenanoscalepossiblycouldshifttheemissionbandstothe lower wavelength, which might be due to a widening induced inthebandgapofthematerial. The PL emission spectra of Ag, Tb, and Cu doped samples shown in Figure 4 (curves (b), (d), and (e)) are almost similartothatofpurecaf 2 (curve (a)), but with a slight PL enhancement. The observed enhancement in case of Ag doped sample might be due to the increase in absorption and quantum yield. This absorption perhaps could be increased duetothesurfaceplasmonresonanceofagions. Ag dopants could perhaps be incorporated in metallic form . It is also possible that some of these dopants could form small clusters; however, this is a preliminary speculation and further investigations are needed to prove the actual nature of Ag as a dopant in CaF 2 host. The emission spectrum of Tb doped sample shows extra band at 544 nm. This band is the well-known emission of Tb 3+ ion, which can be assigned to the 5 D 4 7 F 6 transition of Tb 3+ ion . In case of copper (Cu) ion it is possible that it might get incorporated in the host of LiF matrix in its 2+ form (Cu 2+ ). This ion mostly shows its emission in the visible region. This ion was reported by several authors to have emission bands in the region [43, 44]; therefore, the broad band at nm might include the emission of Cu 2+ andthusshowedplenhancement. The PL emission spectra of Eu and Dy doped samples (Figure 4, curves (c) and (f)) show strong enhancement in intensity of the broad band at nm, with the emergence of extra sharp emissions. The broad band at nm has the highest PL intensity in Eu doped sample. This is in association with emergence of two bands located at 590 and 615 nm, which are the well-known emissions of Eu 3+ ion . Dy ion might get introduced into the host of CaF 2 matrix in its 3+ form (Dy 3+ )andthisionisawellknown activator mostly showing its emission in the visible region. This ion was reported by several authors to have two emissions at around 485 and 572 nm , which are close to the emission region of pure CaF 2.ThefirstemissionofDy 3+ in CaF 2 matrix probably could enhance the PL emission of pure sample by superimposing these emissions. Figure 5 shows the TL glow curves of CaF 2 nanostructures doped with different elements at a concentration of 0.2 mole% (curves (a), (b), (c), (d), and (e)). These samples were exposed to 1 kgy of 137 Cs gamma rays. The glow peaks of Eu, Cu, and Ag dopants (curves (a), (d), and (e)) are located at around 125 C with a version in their relative TL intensity. Tb doped CaF 2 nanostructures (curve (c)) has stronger glow peak at lower temperature side, that is, around 95 C. The Dy doped sample (curve (b)) shows a broad TL glow curve with a prominent peak at around 165 C along with smaller one at 135 C. This curve has the highest TL intensity. This is a remarkable result to have a sensitive material with deeper traps, which is thermally stable with less fading. Moreover, Dy doped CaF 2 sample seems to have a good population of electron traps, making it a good candidate to be tested for its responsetoheavyionsusedinradiotherapylikecarbonions. The nanostructure form of CaF 2 was tested by Zahedifar and Sadeghi [34, 47] and Zahedifar et al. foritsTLresponse TL intensity (a.u.) c e d a b (a) CaF 2 :Eu (b) CaF 2 :Dy (c) CaF 2 :Tb Temperature ( C) (d) CaF 2 :Cu (e) CaF 2 :Ag Figure 5: TL glow curves of CaF 2 nanostructures doped with different elements and exposed to 1 kgy of 137 Cs gamma rays. TL intensity (a.u.) e a 0.05 c TL intensity (a.u.) d Exposure (Gy) b (a) 10 Gy (b) 100 Gy (c) 1 kgy 10 6 Temperature ( C) (d) 10 kgy (e) 30 kgy Figure 6: TL glow curves of CaF 2 :Dy nanostructures exposed to different exposures of 137 Cs gamma rays. The figure in the inset is the corresponding TL response curve. after doping with Tm, Ce. In their sample the permanent glow peak was observed at a relatively low temperature side, which is around 402 K (129 C). This makes CaF 2 :Dy a superior due to its relatively high temperature glow peak. But it is quite useful to test the TL response of CaF 2 :Dy nanostructures to different doses of gamma rays and observe the effect of different doses on the glow curve structure and peak position. Figure 6 shows the TL glow curves of CaF 2 :Dy nanostructures exposed to different exposures of 137 Cs gamma
5 Nanomaterials 5 (a) (b) (c) (d) (e) (f) Figure 7: SEM images of (a) pure and Dy doped nanostructures of CaF2 sample ((b) 0.05, (c) 0.1, (d) 0.2, (e) 1, and (f) 2 mole%). rays in the range of 10 Gy 30 kgy. There is no significant change in the glow curve structure or peak position. The intensity of the glow peaks increased by increasing the dose in the range 10 Gy 10 kgy (curves (a), (b), (c), and (d)), but further exposure beyond this range results in decreasing the TL intensity of the glow peaks (curve (e)). Small TL glow peak emerged at around 70 C in case of 30 kgy exposure, which might be due to the saturation of electrons at the existing electron traps resulting in creating shallow traps. The TL response curve of CaF2 :Dy nanostructures to different exposures of 137 Cs gamma rays was also plotted and presented in the inset of Figure 6. It shows that below 100 Gy the curve is sublinear; then it is quite linear in the range of 100 Gy 10 kgy and finally saturates (even decreases) beyond this range. The linear response in a wide range is good indicator for CaF2 :Dy nanocubes to be tested as a dosimeter for C ions. This wide response was explained earlier by Salah et al. [13, 49]. The effect of Dy concentration on the TL sensitivity of CaF2 nanostructures has been studied. Different concentrations within the range mole% were included in this study. The maximum TL sensitivity was found to be around 0.5 mole%. Strange result was also observed on the particle size of CaF2 nanostructures by changing Dy concentration.
6 6 Nanomaterials Figure 7 shows SEM images at the same magnifications for CaF 2 nanostructures doped with Dy at different concentrations from 0.05 to 2 mole% (images (a) (f)). At low concentration (image (a)) the particle size is around nm. This size was significantly reduced to around 20 nm by increasing concentration of Dy to 2 mole%. Similar results were also observed by Salah  ontbdopedcaso 4 nanorods. The reason for that was attributed to the well incorporation of rareearthionsinthehostthatcouldlimitthegrowthofthese nanostructures; this means that these rare earths ions could act as controlling agents for size growth. The other impurities perhaps could not be incorporated well neither interstitially nor substitutionally. Rare earths like Dy, Tb, and Eu have ionic radii close to that of Ca, while those of Ag and Cu are different. Therefore, these rare earth ions perhaps could substitutionally be incorporated. 4. Conclusion The TL and PL properties of CaF 2 nanostructures doped with Eu, Tb, Dy, Cu, and Ag were studied. Thermally stable nanocrystalline materials with a single phase in the C temperature range could be produced. The PL emission spectrum of pure CaF 2 nanostructureshasabroadbandin therangeof nm.Thedopedsamplesshowedsimilar spectra in addition to extra bands related to these impurities. The maximum PL intensity was observed in Eu doped sample. DydopedonewasobservedtobethemostTLsensitive with a linear response curve in the 100 Gy 10 kgy range. This impurity could also play a role as a controlling agent for particle size growth. These results showed that Dy is a proper activator in the host of CaF 2 nanostructures, providing a highly sensitive dosimeter in a wide range of exposures that might be suitable for measurements of heavy doses. Conflict of Interests The authors declare that there is no conflict of interests regarding the publication of this paper. Acknowledgment Thanks are due to King Abdulaziz City for Science and Technology, Riyadh, Saudi Arabia, for providing financial assistance in the form of Research Project A-T References  B. Nasiri-Tabrizi and A. Fahami, Mechanochemical synthesis and structural characterization of nano-sized amorphous tricalcium phosphate, Ceramics International, vol.39,no.8,pp ,  S. P. Kim, D. U. Lee, and E. K. Kim, Optical properties of metal-oxide nano-particles embedded in the polyimide layer for photovoltaic applications, Current Applied Physics, vol. 10, no. 3, supplement, pp. S478 S480, X.S.Lv,Z.H.Deng,F.X.Miaoetal., Fundamentaloptical andelectricalpropertiesofnano-cu 3 VS 4 thin film, Optical Materials,vol.34,no.8,pp ,2012.  P. Pulišová, J. Kováč, A. Voigt, and P. Raschman, Structure and magnetic properties of Co and Ni nano-ferrites prepared by a two step direct microemulsions synthesis, Magnetism and Magnetic Materials,vol.341,pp.93 99,2013.  V. S. Kortov, Nanophosphors and outlooks for their use in ionizing radiation detection, Radiation Measurements,vol.45, no.3 6,pp ,2010.  C. Wu, W. Qin, G. Qin et al., Photoluminescence from surfactant-assembled Y 2 O 3 :Eu nanotubes, Applied Physics Letters,vol.82,no.4,pp ,2003.  P. R. González, E. Cruz-Zaragoza, C. Furetta, J. Azorín, and B. C. Alcántara, Effect of thermal treatment on TL response of CaSO 4 :Dy obtained using a new preparation method, Applied Radiation and Isotopes,vol.75,pp.58 63,2013.  S. C. Qu, W. H. Zhou, F. Q. Liu et al., Photoluminescence properties of Eu 3+ -doped ZnS nanocrystals prepared in a water/methanol solution, Applied Physics Letters, vol. 80, no. 19,article3605,2002.  M. Isik, E. Bulur, and N. M. Gasanly, TL and TSC studies on TlGaSe 2 layered single crystals, JournalofLuminescence,vol. 144, pp ,  A. Hernandez-Medina, A. Negron-Mendoza, S. Ramos-Bernal, and M. Colin-Garcia, The effect of doses, irradiation temperature, and doped impurities in the thermoluminescence response of NaCl crystals, Radiation Measurements,vol.56,pp ,  J. I. Lee, I. Changa, J. L. Kim et al., LiF:Mg,Cu,Si material with intense high-temperature TL peak prepared by various thermal treatment conditions, Radiation Measurements,vol.46,no.12, pp ,2011.  K.Tang,H.Cui,H.Zhu,Z.Liu,andH.Fan, Newlydeveloped highly sensitive LiF:Mg,Cu,Si TL discs with good stability to heat treatment, Radiation Measurements, vol. 47, no. 2, pp ,  N. Salah, P. D. Sahare, and A. A. Rupasov, Thermoluminescence of nanocrystalline LiF:Mg, Cu, P, Luminescence,vol.124,no.2,pp ,2007.  N. Salah, Carbon ions irradiation on nano- and microcrystalline CaSO 4 :Dy, Physics D: Applied Physics,vol.41, no. 15, Article ID , N.N.Salah,S.S.Habib,Z.H.Khanetal., Nanorodsof LiF:Mg,Cu,P as detectors for mixed field radiations, IEEE Transactions on Nanotechnology,vol.7,no.6,pp ,2008.  N. Salah, S. P. Lochab, D. Kanjilal et al., Nanoparticles of K 2 Ca 2 (SO 4 ) 3 :Eu as effective detectors for swift heavy ions, Applied Physics, vol.102,no.6,articleid064904,  S. P. Lochab, D. Kanjilal, N. Salah et al., Nanocrystalline Ba 0.97 Ca 0.03 SO 4 :Eu for ion beams dosimetry, Applied Physics,vol.104,no.3,article033520,2008.  N. Salah, S. S. Habib, Z. H. Khan, and S. P. Lochab, The nanoparticles of BaSO 4 :Eu as detectors for high doses of different ionising radiations, Atoms for Peace, vol.3,no.2,p. 84,  N. Salah, Nanocrystalline materials for the dosimetry of heavy charged particles: a review, Radiation Physics and Chemistry, vol. 80, no. 1, pp. 1 10,  N. Salah, S. Habib, S. S. Babkair, S. P. Lochab, and V. Chopra, TL response of nanocrystalline MgB 4 O 7 :Dy irradiated by 3 MeV proton beam, 50 MeV Li 3+ and 120 MeV Ag 9+ ion beams, Radiation Physics and Chemistry,vol.86,pp.52 58,2013.
7 Nanomaterials 7  N. Salah, N. D. Alharbi, and M. A. Enani, Luminescence properties of pure and doped CaSO 4 nanorods irradiated by 15 MeV e-beam, Nuclear Instruments and Methods in Physics ResearchSectionB:BeamInteractionswithMaterialsandAtoms, vol. 319, pp ,  V. Kumar, H. C. Swart, O. M. Ntwaeaborwa et al., Thermoluminescence response of CaS:Bi 3+ nanophosphor exposed to 200 MeV Ag +15 ion beam, Optical Materials,vol.32,no.1,pp ,  A. Pandey, S. Bahl, K. Sharm et al., Thermoluminescence properties of nanocrystalline K 2 Ca 2 (SO 4 ) 3 :Euirradiatedwith gamma rays and proton beam, Nuclear Instruments and Methods in Physics Research B,vol.269,no.3,pp ,2011.  A. Choubey, S. K. Sharma, S. P. Lochab, and D. Kanjilal, Excitation of thermoluminescence in Eu doped Ba 0.12 Sr 0.88 SO 4 nanophosphor by low energy argon ions, Luminescence,vol.131,no.10,pp ,2011.  S. C. Prashantha, B. N. Lakshminarasappa, and F. Singh, 100 MeV Si 8+ ion induced luminescence and thermoluminescence of nanocrystalline Mg 2 SiO 4 :Eu 3+, Luminescence,vol. 132, no. 11, pp ,  S. Bahl, A. Pandey, S. P. Lochab, V. E. Aleynikov, A. G. Molokanov, and P. Kumar, Synthesis and thermoluminescence characteristics of gamma and proton irradiated nanocrystalline MgB 4 O 7 :Dy,Na, Luminescence,vol.134,pp ,  C. Manjunatha, D. V. Sunitha, H. Nagabhushana et al., Thermoluminescence properties of 100 MeV Si 7+ swift heavy ions and UV irradiated CdSiO 3 :Ce 3+ nanophosphor, Luminescence,vol.134,pp ,2013.  D. V. Sunitha, H. Nagabhushana, and S. C. Sharma, Structural, iono and thermoluminescence properties of heavy ion (100 MeV Si 7+ )bombardedzn 2 SiO 4 :Sm 3+ nanophosphor, Journal of Luminescence,vol.143,pp ,2013.  C. Pandurangappa and B. Lakshminarasappa, Optical absorption and Photoluminescence studies in Gamma-irradiated nanocrystalline CaF2, Nanomedicine and Nanotechnology, vol. 2, no. 2,  V. Petit, J. L. Doualan, P. Camy, V. Ménard, and R. Moncorgé, CW and tunable laser operation of Yb 3+ doped CaF 2, Applied Physics B,vol.78,no.6,pp ,2004.  G. A. Kumar, C. W. Chen, J. Ballato, and R. E. Riman, Optical characterization of infrared emitting rare-earth-doped fluoride nanocrystals and their transparent nanocomposites, Chemistry of Materials,vol.19,no.6,pp ,2007.  A. Bensalah, M. Mortier, G. Patriarche, P. Gredin, and D. Vivien, Synthesis and optical characterizations of undoped and rare-earth-doped CaF 2 nanoparticles, JournalofSolidState Chemistry, vol. 179, no. 8, pp ,  C. Cao, W. Qin, J. Zhang et al., Up-conversion white light of Tm 3+ /Er 3+ /Yb 3+ tri-doped CaF 2 phosphors, Optics Communications,vol.281,no.6,pp ,2008.  M. Zahedifar and E. Sadeghi, Synthesis and thermoluminescence properties of CaF2: Tm, Ce nanoparticles, Iranian Physics Research,vol.13,no.3,p.55,2013.  D. Chen, Y. Wang, E. Ma, Y. Yu, and F. Liu, Partition, luminescence and energy transfer of Er 3+ /Yb 3+ ions in oxyfluoride glass ceramic containing CaF 2 nano-crystals, Optical Materials,vol. 29, no. 12, pp ,  C. Pandurangappa, B. N. Lakshminarasappa, and B. M. Nagabhushana, Synthesis and optical studies of gamma irradiated Eu doped nanocrystalline CaF 2, Alloys and Compounds, vol. 509, no. 29, pp ,  J. Tao, Q. Weiping, and Z. Dan, Size-dependent upconversion luminescence in CaF 2 :Yb 3+,Tm 3+ nanocrystals, Materials Letters,vol.74,pp.54 57,2012.  Y.Li,T.Liu,andY.Du, Acceleratedfabricationandupconversion luminescence of Yb 3+ /Er 3+ -codoped CaF 2 nanocrystal by microwave heating, Applied Physics Express,vol.5,no.8,Article ID ,  F. Somma, R. M. Montereali, M. A. Vincenti, S. Polosan, and M. Secu, Radiation induced defects in Pb +2 -doped LiF crystals, Physics Procedia,vol.2,no.2,pp ,2009.  M. Darroudi, M. B. Ahmad, A. H. Abdullah, N. A. Ibrahim, and K. Shameli, Effect of accelerator in green synthesis of silver nanoparticles, International Molecular Sciences, vol. 11, no. 10, pp , Y.Chen,X.L.Xu,G.H.Zhang,H.Xue,andS.Y.Ma, A comparative study of the microstructures and optical properties of Cu- and Ag-doped ZnO thin films, PhysicaB:Condensed Matter,vol.404,no.20,pp ,2009.  S. Sato, S. Kamei, K. Uematsu et al., Synthesis and luminescence properties of rare earth doped Na 3 AlP 3 O 9 N oxynitridophosphate phosphor, Ceramic Processing Research, vol.14,no.1,pp.s74 s76,2013.  W.-C. Lin, C.-Y. Wu, Z.-H. Liu, C.-Y. Lin, and Y.-P. Yen, A new selective colorimetric and fluorescent sensor for Hg 2+ and Cu 2+ based on a thiourea featuring a pyrene unit, Talanta,vol.81,no. 4-5, pp , N.Li,Y.Xiang,andA.Tong, Highlysensitiveandselective turn-on fluorescent chemodosimeter for Cu 2+ in water via Cu 2+ -promoted hydrolysis of lactone moiety in coumarin, Chemical Communications,vol.46,no.19,pp ,2010.  K. Sivaiah and S. Buddhudu, Light-emission in Tb 3+ and Eu 3+ : PVP polymer films, Indian Pure and Applied Physics, vol. 49, no. 6, pp , Y.-C.Li,Y.-H.Chang,Y.-F.Lin,Y.-S.Chang,andY.-J.Lin, Synthesis and luminescent properties of Ln 3+ (Eu 3+,Sm 3+, Dy 3+ )-doped lanthanum aluminum germanate LaAlGe 2 O 7 phosphors, Alloys and Compounds,vol.439,no.1-2, pp ,  M. Zahedifar and E. Sadeghi, Synthesis and dosimetric properties of the novel thermoluminescent CaF 2 :Tm nanoparticles, Radiation Physics and Chemistry, vol.81,no.12,pp ,  M. Zahedifar, E. Sadeghi, and Z. Mohebbi, Synthesis and thermoluminescence characteristics of Mn doped CaF 2 nanoparticles, Nuclear Instruments and Methods in Physics Research, Section B: Beam Interactions with Materials and Atoms,vol.274, pp ,2012.  N. Salah, Z. H. Khan, and S. S. Habib, Copper activated LiF nanorods as TLD material for high exposures of gamma-rays, Nuclear Instruments and Methods in Physics Research Section B: Beam Interactions with Materials and Atoms,vol.267,no.21-22, pp ,  N. Salah, Thermoluminesence of gamma rays irradiated CaSO 4 nanorods doped with different elements, Radiation Physics and Chemistry,vol.106,pp.40 45,2015.
8 Nanotechnology International International Corrosion Polymer Science Smart Materials Research Composites Metallurgy BioMed Research International Nanomaterials Submit your manuscripts at Materials Nanoparticles Nanomaterials Advances in Materials Science and Engineering Nanoscience Scientifica Coatings Crystallography The Scientific World Journal Textiles Ceramics International Biomaterials